General

Property | Value | Temperature |
---|---|---|

Density | 7.85 g/cm³ Show Material materials with Density of 7.85 g/cm³ at 20.0 °C | 20.0 °C |

Mechanical

Property | Value | Temperature |
---|---|---|

Elastic modulus | 217 GPa Show Material materials with Elastic modulus of 217 GPa at -100.0 °C | -100.0 °C |

210 - 212 GPa Show Material materials with Elastic modulus of 210 - 212 GPa at 20.0 °C | 20.0 °C | |

205 - 207 GPa Show Material materials with Elastic modulus of 205 - 207 GPa at 100.0 °C | 100.0 °C | |

193 - 199 GPa Show Material materials with Elastic modulus of 193 - 199 GPa at 200.0 °C | 200.0 °C | |

185 - 192 GPa Show Material materials with Elastic modulus of 185 - 192 GPa at 300.0 °C | 300.0 °C | |

175 - 184 GPa Show Material materials with Elastic modulus of 175 - 184 GPa at 400.0 °C | 400.0 °C | |

175 GPa Show Material materials with Elastic modulus of 175 GPa at 500.0 °C | 500.0 °C | |

164 GPa Show Material materials with Elastic modulus of 164 GPa at 600.0 °C | 600.0 °C | |

Elongation | 8 - 12 % Show Material materials with Elongation of 8 - 12 % at 20.0 °C | 20.0 °C |

Poisson's ratio | 0.28 [-] Show Material materials with Poisson's ratio of 0.28 [-] at 20.0 °C | 20.0 °C |

Shear modulus | 81 GPa Show Material materials with Shear modulus of 81 GPa at 20.0 °C | 20.0 °C |

Tensile strength | 320 - 760 MPa Show Material materials with Tensile strength of 320 - 760 MPa at 20.0 °C | 20.0 °C |

Yield strength Rp0.2 | 180 - 350 MPa Show Material materials with Yield strength Rp0.2 of 180 - 350 MPa at 20.0 °C | 20.0 °C |

Thermal

Property | Value | Temperature | Comment |
---|---|---|---|

Coefficient of thermal expansion | 1.08E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.08E-5 1/K at -100.0 °C | -100.0 °C | |

1.19E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.19E-5 1/K at 20.0 °C | 20.0 °C | ||

1.1E-5 - 1.25E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.1E-5 - 1.25E-5 1/K at 100.0 °C | 100.0 °C | ||

1.18E-5 - 1.3E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.18E-5 - 1.3E-5 1/K at 200.0 °C | 200.0 °C | ||

1.36E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.36E-5 1/K at 300.0 °C | 300.0 °C | ||

1.32E-5 - 1.41E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.32E-5 - 1.41E-5 1/K at 400.0 °C | 400.0 °C | ||

1.45E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.45E-5 1/K at 500.0 °C | 500.0 °C | ||

1.49E-5 1/K Show Material materials with Coefficient of thermal expansion of 1.49E-5 1/K at 600.0 °C | 600.0 °C | ||

Unlock all property charts | |||

Max service temperature | 500 °C Show Material materials with Max service temperature of 500 °C | Typical for Carbon Steel | |

Max service temperature, long | -25 - 0 °C Show Material materials with Max service temperature, long of -25 - 0 °C | ||

Melting point | 1480 - 1526 °C Show Material materials with Melting point of 1480 - 1526 °C | Typical for Low Carbon Steel | |

Specific heat capacity | 423 J/(kg·K) Show Material materials with Specific heat capacity of 423 J/(kg·K) at -100.0 °C | -100.0 °C | |

460 - 461 J/(kg·K) Show Material materials with Specific heat capacity of 460 - 461 J/(kg·K) at 20.0 °C | 20.0 °C | ||

479 - 480 J/(kg·K) Show Material materials with Specific heat capacity of 479 - 480 J/(kg·K) at 100.0 °C | 100.0 °C | ||

499 - 520 J/(kg·K) Show Material materials with Specific heat capacity of 499 - 520 J/(kg·K) at 200.0 °C | 200.0 °C | ||

517 J/(kg·K) Show Material materials with Specific heat capacity of 517 J/(kg·K) at 300.0 °C | 300.0 °C | ||

536 J/(kg·K) Show Material materials with Specific heat capacity of 536 J/(kg·K) at 400.0 °C | 400.0 °C | ||

558 J/(kg·K) Show Material materials with Specific heat capacity of 558 J/(kg·K) at 500.0 °C | 500.0 °C | ||

587 J/(kg·K) Show Material materials with Specific heat capacity of 587 J/(kg·K) at 600.0 °C | 600.0 °C | ||

Unlock all property charts | |||

Thermal conductivity | 57.5 - 58.7 W/(m·K) Show Material materials with Thermal conductivity of 57.5 - 58.7 W/(m·K) at 20.0 °C | 20.0 °C | |

54.4 - 55.7 W/(m·K) Show Material materials with Thermal conductivity of 54.4 - 55.7 W/(m·K) at 100.0 °C | 100.0 °C | ||

50.2 - 51.9 W/(m·K) Show Material materials with Thermal conductivity of 50.2 - 51.9 W/(m·K) at 200.0 °C | 200.0 °C | ||

47.6 W/(m·K) Show Material materials with Thermal conductivity of 47.6 W/(m·K) at 300.0 °C | 300.0 °C | ||

43.4 - 44 W/(m·K) Show Material materials with Thermal conductivity of 43.4 - 44 W/(m·K) at 400.0 °C | 400.0 °C | ||

39.6 W/(m·K) Show Material materials with Thermal conductivity of 39.6 W/(m·K) at 500.0 °C | 500.0 °C | ||

36 W/(m·K) Show Material materials with Thermal conductivity of 36 W/(m·K) at 600.0 °C | 600.0 °C | ||

Unlock all property charts | |||

Thermal diffusivity | 15.9 mm²/s Show Material materials with Thermal diffusivity of 15.9 mm²/s at 20.0 °C | 20.0 °C | |

14.3 mm²/s Show Material materials with Thermal diffusivity of 14.3 mm²/s at 100.0 °C | 100.0 °C | ||

12.5 mm²/s Show Material materials with Thermal diffusivity of 12.5 mm²/s at 200.0 °C | 200.0 °C | ||

10.8 mm²/s Show Material materials with Thermal diffusivity of 10.8 mm²/s at 300.0 °C | 300.0 °C | ||

9.2 mm²/s Show Material materials with Thermal diffusivity of 9.2 mm²/s at 400.0 °C | 400.0 °C | ||

7.6 mm²/s Show Material materials with Thermal diffusivity of 7.6 mm²/s at 500.0 °C | 500.0 °C | ||

6.1 mm²/s Show Material materials with Thermal diffusivity of 6.1 mm²/s at 600.0 °C | 600.0 °C | ||

Unlock all property charts |

Electrical

Property | Value | Temperature |
---|---|---|

Electrical resistivity | 1.1E-7 Ω·m Show Material materials with Electrical resistivity of 1.1E-7 Ω·m at 20.0 °C | 20.0 °C |

2.3E-7 Ω·m Show Material materials with Electrical resistivity of 2.3E-7 Ω·m at 100.0 °C | 100.0 °C | |

3.04E-7 Ω·m Show Material materials with Electrical resistivity of 3.04E-7 Ω·m at 200.0 °C | 200.0 °C | |

3.94E-7 Ω·m Show Material materials with Electrical resistivity of 3.94E-7 Ω·m at 300.0 °C | 300.0 °C | |

5.01E-7 Ω·m Show Material materials with Electrical resistivity of 5.01E-7 Ω·m at 400.0 °C | 400.0 °C | |

6.25E-7 Ω·m Show Material materials with Electrical resistivity of 6.25E-7 Ω·m at 500.0 °C | 500.0 °C | |

7.7E-7 Ω·m Show Material materials with Electrical resistivity of 7.7E-7 Ω·m at 600.0 °C | 600.0 °C | |

Unlock all property charts |

Magnetic

Property | Value | Comment |
---|---|---|

Curie temperature | 770 °C Show Material materials with Curie temperature of 770 °C | Typical for Low Carbon Steel |

Chemical properties

Property | ||
---|---|---|

Carbon | 0.07 - 0.13 % | |

Manganese | 0.3 - 0.6 % | |

Phosphorus | 0.05 % | |

Silicon | 0.4 % | |

Sulfur | 0.045 % |